General

Property | Value | Condition | Related Standards | Shape |
---|---|---|---|---|

Density | 2.77 g/cm³ Show Material materials with Density of 2.77 g/cm³ | T351 | ||

2.78 g/cm³ Show Material materials with Density of 2.78 g/cm³ | T351 | AA Standards, ASTM B209, ASTM B211 | ||

2.78 g/cm³ Show Material materials with Density of 2.78 g/cm³ | T351 | |||

2.79 g/cm³ Show Material materials with Density of 2.79 g/cm³ | T351 | Bar | ||

3.0 g/cm³ Show Material materials with Density of 3.0 g/cm³ | T351 |

Mechanical

Property | Temperature | Value | Condition | Related Standards | Shape | Comment |
---|---|---|---|---|---|---|

Elastic modulus | 72.4 GPa Show Material materials with Elastic modulus of 72.4 GPa | T351 | ||||

73.0 GPa Show Material materials with Elastic modulus of 73.0 GPa | T351 | AA Standards, ASTM B209, ASTM B211 | Bar | |||

73 GPa Show Material materials with Elastic modulus of 73 GPa | T351 | |||||

Elongation | -195 °C | 19 % Show Material materials with Elongation of 19 % | T351 | Elongation in 50 mm | ||

-80 °C | 19 % Show Material materials with Elongation of 19 % | T351 | Elongation in 50 mm | |||

3.0 % Show Material materials with Elongation of 3.0 % | T351 | AA Standards, ASTM B209 | A100 | |||

5.0 % Show Material materials with Elongation of 5.0 % | T351 | AA Standards, ASTM B209 | A100 | |||

6.0 % Show Material materials with Elongation of 6.0 % | T351 | AA Standards, ASTM B209 | A100 | |||

7.0 % Show Material materials with Elongation of 7.0 % | T351 | AA Standards, ASTM B209 | A100 | |||

8.0 % Show Material materials with Elongation of 8.0 % | T351 | AA Standards, ASTM B211 | A100 | |||

9.0 % Show Material materials with Elongation of 9.0 % | T351 | AA Standards, ASTM B211 | A100 | |||

10.0 % Show Material materials with Elongation of 10.0 % | T351 | Bar | A50 | |||

12.0 % Show Material materials with Elongation of 12.0 % | T351 | AA Standards, ASTM B209 | A50 | |||

13.0 % Show Material materials with Elongation of 13.0 % | T351 | |||||

0 °C | 19 % Show Material materials with Elongation of 19 % | T351 | Elongation in 50 mm | |||

20.0 % Show Material materials with Elongation of 20.0 % | T351 | |||||

24 °C | 19 % Show Material materials with Elongation of 19 % | T351 | Elongation in 50 mm | |||

100 °C | 19 % Show Material materials with Elongation of 19 % | T351 | Elongation in 50 mm | |||

150 °C | 17 % Show Material materials with Elongation of 17 % | T351 | Elongation in 50 mm | |||

205 °C | 27 % Show Material materials with Elongation of 27 % | T351 | Elongation in 50 mm | |||

260 °C | 55 % Show Material materials with Elongation of 55 % | T351 | Elongation in 50 mm | |||

315 °C | 75 % Show Material materials with Elongation of 75 % | T351 | Elongation in 50 mm | |||

370 °C | 100 % Show Material materials with Elongation of 100 % | T351 | Elongation in 50 mm | |||

Plane-Strain Fracture Toughnes | 26 MPa·√m Show Material materials with Plane-Strain Fracture Toughnes of 26 MPa·√m | T351 | For plate in T-L direction | |||

Poisson's ratio | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | T351 | ||||

Shear modulus | 28.0 GPa Show Material materials with Shear modulus of 28.0 GPa | T351 | ||||

Tensile strength | -195 °C | 580 MPa Show Material materials with Tensile strength of 580 MPa | T351 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | ||

-80 °C | 490 MPa Show Material materials with Tensile strength of 490 MPa | T351 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | |||

395.0 MPa Show Material materials with Tensile strength of 395.0 MPa | T351 | AA Standards, ASTM B209 | ||||

415.0 MPa Show Material materials with Tensile strength of 415.0 MPa | T351 | AA Standards, ASTM B209 | ||||

425.0 MPa Show Material materials with Tensile strength of 425.0 MPa | T351 | AA Standards, ASTM B209, ASTM B211 | ||||

427.0 MPa Show Material materials with Tensile strength of 427.0 MPa | T351 | Bar | ||||

435.0 MPa Show Material materials with Tensile strength of 435.0 MPa | T351 | AA Standards, ASTM B209 | ||||

440.0 MPa Show Material materials with Tensile strength of 440.0 MPa | T351 | AA Standards, ASTM B209 | ||||

470.0 MPa Show Material materials with Tensile strength of 470.0 MPa | T351 | |||||

0 °C | 475 MPa Show Material materials with Tensile strength of 475 MPa | T351 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | |||

24 °C | 470 MPa Show Material materials with Tensile strength of 470 MPa | T351 | ||||

100 °C | 435 MPa Show Material materials with Tensile strength of 435 MPa | T351 | ||||

150 °C | 310 MPa Show Material materials with Tensile strength of 310 MPa | T351 | ||||

205 °C | 180 MPa Show Material materials with Tensile strength of 180 MPa | T351 | ||||

260 °C | 75 MPa Show Material materials with Tensile strength of 75 MPa | T351 | ||||

315 °C | 52 MPa Show Material materials with Tensile strength of 52 MPa | T351 | ||||

370 °C | 35 MPa Show Material materials with Tensile strength of 35 MPa | T351 | ||||

Yield strength | -80 °C | 338 MPa Show Material materials with Yield strength of 338 MPa | T351 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | ||

285.0 MPa Show Material materials with Yield strength of 285.0 MPa | T351 | AA Standards, ASTM B209 | RP02 | |||

290.0 MPa Show Material materials with Yield strength of 290.0 MPa | T351 | AA Standards, ASTM B209 | RP02 | |||

310.0 MPa Show Material materials with Yield strength of 310.0 MPa | T351 | AA Standards, ASTM B211 | Bar | RP02 | ||

0 °C | 324 MPa Show Material materials with Yield strength of 324 MPa | T351 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | |||

325.0 MPa Show Material materials with Yield strength of 325.0 MPa | T351 | |||||

330.0 MPa Show Material materials with Yield strength of 330.0 MPa | T351 | |||||

24 °C | 324 MPa Show Material materials with Yield strength of 324 MPa | T351 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | |||

100 °C | 310 MPa Show Material materials with Yield strength of 310 MPa | T351 | ||||

150 °C | 248 MPa Show Material materials with Yield strength of 248 MPa | T351 | ||||

205 °C | 131 MPa Show Material materials with Yield strength of 131 MPa | T351 | ||||

260 °C | 62 MPa Show Material materials with Yield strength of 62 MPa | T351 | ||||

315 °C | 41 MPa Show Material materials with Yield strength of 41 MPa | T351 | ||||

370 °C | 28 MPa Show Material materials with Yield strength of 28 MPa | T351 |

Thermal

Property | Temperature | Value | Condition | Shape | Related Standards |
---|---|---|---|---|---|

Coefficient of thermal expansion | 2.29e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.29e-05 1/K | T351 | |||

2.3e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.3e-05 1/K | T351 | ||||

2.31e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.31e-05 1/K | T351 | Bar | |||

20 °C | 2.3199999999999998e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.3199999999999998e-05 1/K | T351 | AA Standards, ASTM B209, ASTM B211 | ||

100 °C | 2.3199999999999998e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.3199999999999998e-05 1/K | T351 | AA Standards, ASTM B209, ASTM B211 | ||

Melting point | 500.0 °C Show Material materials with Melting point of 500.0 °C | T351 | |||

505.0 - 635.0 °C Show Material materials with Melting point of 505.0 - 635.0 °C | T351 | AA Standards, ASTM B209, ASTM B211 | |||

640.0 °C Show Material materials with Melting point of 640.0 °C | T351 | Bar | |||

Specific heat capacity | 870.0 J/(kg·K) Show Material materials with Specific heat capacity of 870.0 J/(kg·K) | T351 | |||

875.0 J/(kg·K) Show Material materials with Specific heat capacity of 875.0 J/(kg·K) | T351 | ||||

Thermal conductivity | 120.0 W/(m·K) Show Material materials with Thermal conductivity of 120.0 W/(m·K) | T351 | |||

121.0 - 193.0 W/(m·K) Show Material materials with Thermal conductivity of 121.0 - 193.0 W/(m·K) | T351 | AA Standards, ASTM B209, ASTM B211 | |||

121.0 - 150.0 W/(m·K) Show Material materials with Thermal conductivity of 121.0 - 150.0 W/(m·K) | T351 | Bar |

Electrical

Property | Value | Condition | Related Standards | Shape | Comment |
---|---|---|---|---|---|

Electrical conductivity | 17000000.0 - 29000000.0 S/m Show Material materials with Electrical conductivity of 17000000.0 - 29000000.0 S/m | T351 | AA Standards, ASTM B209, ASTM B211 | ||

Electrical resistivity | 3.45e-08 - 5.88e-08 Ω·m Show Material materials with Electrical resistivity of 3.45e-08 - 5.88e-08 Ω·m | T351 | AA Standards, ASTM B209, ASTM B211 | ||

4.31e-08 - 5.75e-08 Ω·m Show Material materials with Electrical resistivity of 4.31e-08 - 5.75e-08 Ω·m | T351 | Bar | |||

5.7e-08 Ω·m Show Material materials with Electrical resistivity of 5.7e-08 Ω·m | T351 | Typical value |

Chemical properties

Property | Value | Condition | Related Standards | Shape | Comment |
---|---|---|---|---|---|

Aluminium | 90.7 - 94.7 % Show Material materials with Aluminium of 90.7 - 94.7 % | T351 | |||

Chromium | 0.1 % Show Material materials with Chromium of 0.1 % | T351 | AA Standards, ASTM B209, ASTM B211 | Bar | |

Copper | 3.8 - 4.9 % Show Material materials with Copper of 3.8 - 4.9 % | T351 | AA Standards, ASTM B209, ASTM B211 | Bar | |

Iron | 0.50 % Show Material materials with Iron of 0.50 % | T351 | AA Standards, ASTM B209, ASTM B211 | ||

0.5 % Show Material materials with Iron of 0.5 % | T351 | Bar | |||

Magnesium | 1.2 - 1.8 % Show Material materials with Magnesium of 1.2 - 1.8 % | T351 | AA Standards, ASTM B209, ASTM B211 | Bar | |

Manganese | 0.3 - 0.9 % Show Material materials with Manganese of 0.3 - 0.9 % | T351 | AA Standards, ASTM B209, ASTM B211 | Bar | |

Other | 0.15 % Show Material materials with Other of 0.15 % | T351 | Bar | Total | |

Silicon | 0.5 % Show Material materials with Silicon of 0.5 % | T351 | AA Standards, ASTM B209, ASTM B211 | Bar | |

Titanium | 0.15 % Show Material materials with Titanium of 0.15 % | T351 | AA Standards, ASTM B209, ASTM B211 | Bar | |

Zinc | 0.25 % Show Material materials with Zinc of 0.25 % | T351 | AA Standards, ASTM B209, ASTM B211 | Bar | |

Zirconium | 0.2 % Show Material materials with Zirconium of 0.2 % | T351 | Bar | Ti + Zr |

Technological properties

Property | ||
---|---|---|

Application areas | Aerospace | |

Brazing | general: no brazing is known or developed | |

Corrosion properties | Stress corrosion cracking: Betriebsschäden in Gebieten mit Zugspannungen quer zur Kornstruktur, Eingeschränkte Schäden an Laborproben (T4,T3, T351, T3510, T3511), d (T6, T861, T81, T851, T8510, T8511), general: sufficient, in principle it should be protected | |

General machinability | General: poor (O), good to acceptable | |

Workability | general (condition): poor(T4, T3, T351, T3510, T3511, T6), not suitable (T361, T861, T81, T851, T8510, T8511) |